advertisement

Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 Phil. Trans. R. Soc. A (2012) 370, 1871–1895 doi:10.1098/rsta.2011.0429 On longitudinal compressive failure of carbon-ﬁbre-reinforced polymer: from unidirectional to woven, and from virgin to recycled BY S. T. PINHO*, R. GUTKIN, S. PIMENTA, N. V. DE CARVALHO AND P. R OBINSON Department of Aeronautics, Imperial College London, South Kensington, London SW7 2AZ, UK Modelling the longitudinal compressive failure of carbon-ﬁbre-reinforced composites has been attempted for decades. Despite many developments, no single model has surfaced to provide simultaneously a deﬁnitive explanation for the micromechanics of failure as well as validated predictions for a generic stress state. This paper explores the reasons for this, by presenting experimental data (including scanning electron microscopic observations of loaded kink bands during propagation, and brittle shear fracture at 45◦ to the ﬁbres) and reviewing previously proposed micromechanical analytical and numerical models. The paper focuses mainly on virgin unidirectional (UD) composites, but studies for woven and recycled composites are also presented, highlighting similarities and differences between these cases. It is found that, while kink-band formation (also referred to in the literature as microbuckling) is predominant in UD composites under longitudinal compression, another failure mode related to the failure of the ﬁbres can be observed experimentally. It is also shown that the micromechanics of the failure process observed in UD composites is similar to that in other ﬁbre architectures, hence encouraging the adaptation and application of models developed for the former to the latter. Keywords: kink band; composite; fracture; unidirectional; woven; recycled 1. Introduction Longitudinal compressive failure has been a topic of research for several decades because of its signiﬁcance in structural design. Different models have been proposed, based on microbuckling of the ﬁbres [1] and on ﬁbre kinking [2] (ﬁgure 1). Key developments to these theories have been put forward more recently [5–7]. Figure 1c shows failure predictions for longitudinal loading (s11 ) combined with in-plane shear (t12 ) for several models (polynomial, e.g. Tsai–Wu and maximum stress; physically based, e.g. Puck and LaRC05); see the study of Gutkin et al. [4] for a discussion. *Author for correspondence ([email protected]). One contribution of 15 to a Theme Issue ‘Geometry and mechanics of layered structures and materials’. 1871 This journal is © 2012 The Royal Society Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1872 S. T. Pinho et al. (a) (b) (c) b a w Tsai–Wu LaRC05 – linear Puck –1.2 –1.0 –0.8 maximum stress LaRC05 – nonlinear –0.6 s11/XC –0.4 –0.2 t12/SL 1.2 1.0 0.8 0.6 0.4 0.2 0 Figure 1. (a) Micrograph of a kink band. (b) Typical kink-band geometrical parameters (a, ﬁbre orientation; b, band orientation; w, band width) [3]. (c) Failure envelope under combined longitudinal compression and shear; the longitudinal and shear stresses are non-dimensionalized by their respective strength XC and SL [4]. The experimental, numerical and analytical results presented in this paper highlight the physical processes underlying longitudinal compressive failure for a range of composites, focusing mainly on unidirectional (UD) composites (§2). Section 2a introduces experimental observations and ﬁnite-element (FE) micromechanical modelling results that support the development of a model for ﬁbre kinking under pure longitudinal compression (also presented). Section 2b uses a similar approach to analyse kink-band formation for longitudinal compression superposed with in-plane shear. The two approaches complement each other, with the ﬁrst one based on a plasticity model suitable for ductile resins, while the second one is based on principles of ﬁnite fracture mechanics more suited to brittle resins. Section 2c ﬁnally investigates a different failure mode under longitudinal compression: shear-driven ﬁbre compressive failure. Similar work for woven composites is presented in §3 and for recycled composites in §4. The relation between the compressive failure mechanisms is discussed in §5 and conclusions are drawn in §6. 2. The physics of ﬁbre kinking in unidirectional plies (a) Pure longitudinal compression (i) Experimental observations Using scanning electron microscopy, observations of loaded kink bands during propagation (ﬁgure 2; see also [8]) reveal how their formation is related to the development of microcracks in the matrix (label ‘m’ in ﬁgure 2c), which can coalesce into splits (label ‘c’ in ﬁgure 2c), and with ﬁbre failure appearing only relatively late in the process. Carbon ﬁbres eventually fracture because of the formation of shear bands (ﬁgure 3). It will be noted in §2c that shear-dominated ﬁbre failure can also lead to another failure mode at the ply level, entirely different from ﬁbre kinking. (ii) Micromechanical ﬁnite-element modelling In order to complement the qualitative experimental data detailed in §2a(i) and gather quantitative insight on local stress and displacement ﬁelds, Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1873 Longitudinal compressive failure of CFRP (a) kink-band tip (b) kink-band propagation 1 mm (b) ‘c’ (c) ‘m’ fibre 90 µm matrix 20µm Figure 2. (a) Kink band propagating from right to left. (b) Damage and localization are visible ahead of the fully formed kink band. (c) Damage in the matrix and interface [8]. 1 2 2 ‘c’ 1 matrix fibre 20 µm 6 µm 5µm Figure 3. Failure mode of carbon ﬁbres during kinking: shear bands form on the side of higher compressive stress at an angle approximately 45◦ with the longitudinal ﬁbre direction [8]. kink-band formation and propagation were simulated using two-dimensional micromechanical FE models [3]. Several modelling approaches have been used: the initial geometry of the ﬁbres was either sinusoidal or perfectly straight (ﬁgure 4), and different constitutive laws were investigated—cohesive or plastic formulations for the matrix, and elastic or failing ﬁbre response. The load versus displacement curves and the stress ﬁelds obtained (ﬁgure 5) can be correlated with the sequence of events during kink-band formation: matrix failure occurs immediately prior to the peak load, and ﬁbre failure takes Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1874 S. T. Pinho et al. (a) L = 750 µm (b) L = 750µm 100 fibres 50 sinusoidal fibres 150 perfect fibres matrix fibre Figure 4. Micromechanical FE models for the simulation of kink bands, highlighting the initial shape of every 10th ﬁbre: (a) baseline model with mesh detail; (b) model for kink-band propagation into the initially defect-free ﬁbres [3]. (a) (b) fibre axial stresses onset of fibre failure propagation 6 P (N mm–1) matrix shear stresses 4 2 y (µm) 0 50 100 y (µm) 150 onset of matrix yielding Figure 5. The sequence of events for ﬁbre kinking from the FE micromechanical models [3]. (a) Load P versus ﬁbre deﬂection y (baseline FE model). Triangle, onset of matrix yielding; circle, deﬁnition of a full yield band; plus symbol, onset of outer ﬁbre failure; cross symbol, onset of central ﬁbre failure. (b) Stress ﬁelds in defect-free ﬁbres during kink-band propagation. (Online version in colour.) place only much later (on the side of higher compressive stress), after most of the load-bearing capability has been lost. These results are supported by the experimental evidence in ﬁgure 3; in addition, the ﬁbre displacement ﬁelds obtained numerically compare well with those observed in specimens (ﬁgure 6). Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1875 Longitudinal compressive failure of CFRP (a) (b) 200 µm µm Figure 6. Fibre deﬂection during kink-band propagation: comparison between FE micromechanical models and experimental results [3]. (a) Fibre deﬂection predicted with the FE model with initially straight ﬁbres. (b) Fibre deﬂection observed experimentally during kink-band propagation (specimen under load). (a) y q y (b) P t y M P y0 L/2 dy M yT x,u L du fibres matrix dx u Figure 7. Development of the analytical model for kink-band formation under pure longitudinal compression [9]. (a) Equilibrium diagram for the ﬁbre on an elasto-plastic matrix. (b) Deﬁnition of matrix shear strains in the elastic domain. (iii) Analytical modelling An analytical model has been developed [9] to represent the mechanisms of kink-band formation under pure longitudinal compression, as observed experimentally (§2a(i)) and numerically (§2a(ii)). The model is based on the equilibrium of a ﬁbre with a sinusoidal imperfection (y0 ) along the length L. Under longitudinal compression (load P), the ﬁbre bends (deﬂection y and deformed shape yT ), while being supported in shear (stresses t) by an elasto-plastic matrix (ﬁgure 7a). Before the onset of matrix yielding, adjacent ﬁbres are assumed to deform in-phase (IP); therefore, at each point x along the imperfection length, elastic shear strains in the matrix layers are related to the deformation of the ﬁbre (deﬂection y, rotation q and longitudinal displacement u in ﬁgure 7b). The onset of matrix yielding deﬁnes the peak load and the transition to a softening domain, during which a central band of perfectly plastic matrix grows as compression proceeds; the kink band is considered to be fully formed when ﬁbre stresses sf locally reach the ﬁbre compressive strength XCf . The analytical model predicts the load versus displacement curve and the deﬂection and stress ﬁelds accurately; the main events for kink-band formation are predicted by the model, and a good quantitative correlation with FE results Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1876 S. T. Pinho et al. (a) (b) softening domain (point in (a)) 1600 6 800 4 sf (MPa) P (N mm–1) 1200 400 2 elastic domain (point in (a)) 0 x L –400 0 50 100 y (µm) 150 200 –800 Figure 8. Results from the analytical model for kink-band formation under pure longitudinal compression [9]. (a) Load P versus ﬁbre deﬂection y from the analytical model. Triangle, onset of matrix yielding; circle, deﬁnition of a full yield band; cross symbol, onset of ﬁbre failure; ﬁlled square, elastic domain (ﬁbre stresses in (b)); ﬁlled diamond, softening domain (ﬁbre stresses in (b)). (b) Maximum ﬁbre stresses sf along the ﬁbre: analytical (solid lines) versus FE (dashed lines) results. is also achieved (ﬁgure 8). Moreover, the analytical model leads to a closedform prediction of strength as a function of initial misalignments, and to the computation of the kink-band width at the onset of ﬁbre failure [9]. (b) Combined compression and shear (i) Experimental observations Experimental failure envelopes for longitudinal compression and in-plane shear are not always easy to interpret because of signiﬁcant scatter (ﬁgure 9). However, it is apparent that different envelopes follow different trends: while the envelopes in ﬁgure 9a,b appear to be divided into two regions with two different slopes, the envelope shown in ﬁgure 9c appears to be characterized by only one (perhaps straight) segment, while in ﬁgure 9d, the scatter is too large to extract a reasonable trend. Therefore, ﬁgure 9 raises two questions: Why do similar materials follow different trends? Could the two apparent segments observed in certain envelopes correspond to two different failure modes? (ii) Micromechanical ﬁnite-element modelling To gain insight on the mechanisms involved in the failure envelopes shown in ﬁgure 9, micromechanical FE models have been developed. The FE model, shown in ﬁgure 10, shares similarities with those from §2a(ii), but because of the large number of simulations required to generate the failure envelopes, a unit cell of a matrix layer between two half-ﬁbres is preferred. Periodic boundary conditions have been applied to the model to represent actual conditions in the Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1877 Longitudinal compressive failure of CFRP (b) 1.5 1.0 1.0 t12/SL 1.5 0.5 t12/SL (a) 0.5 (c) (d ) 1.5 1.0 1.0 t12/SL t12/SL 1.5 0.5 0.5 –1.5 –1.0 –0.5 0 –1.5 –1.0 –0.5 0 s11/XC s11/XC Figure 9. Comparison of failure envelopes for longitudinal compression with in-plane shear, measured by four different research groups, showing high scatter and different trends [4]. Original data from earlier studies [10–13]. (a) Carbon/epoxy; (b) carbon/epoxy (T300/914C); (c) carbon/epoxy EXAS HST/DX 6002); and (d) carbon/vinyl ester. half-fibre (i,d)(i+1,d) q0 (i,0)(i+1,0) matrix shear shear periodic boundary conditions (0,0) compression L/2 2, y L 1, x Figure 10. Micromechanical FE model with periodic boundary conditions. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1878 S. T. Pinho et al. (a) (b) elastic perfectly plastic; tY = 100 MPa 100 80 60 40 20 –2000 –1500 –1000 s11 (MPa) –500 0 100 q0 = 0.5°, XCf = 3200 MPa 80 60 q0 = 0°, XCf = 6400 MPa –4500 –3500 q0 = 0°, XCf = 3200 MPa 40 q0 = 2°, XCf = 3200 MPa –2500 –1500 s11 (MPa) –500 t12 (MPa) 120 t12 (MPa) nonlinear elasto-plastic elastic perfectly plastic; tY = 90 MPa 20 0 Figure 11. (a) Bimodal failure envelopes obtained using micromechanical FE models, highlighting the sensitivity to matrix constitutive properties. (b) Failure envelopes highlighting the sensitivity to ﬁbre properties [4]. composite; the nodes on each top and bottom external boundary of the half-ﬁbres are constrained so that their displacements in the x and y directions (u, v) follow ∀x ∈ [0, L] : u(x, y = d) = u(x, y = 0), v(x, y = d) = v(x, y = 0) − V , (2.1) where V accounts for Poisson’s expansion in the y direction, and d is the dimension of the unit cell in the y direction. The model is then subjected to several combinations of longitudinal compression and in-plane shear [4]. The softening induced by matrix microcracking is represented using an elastic–plastic constitutive law for the matrix layer (with a yield strength tY ) and the ﬁbres use a continuum damage model, where the stress carried by a ﬁbre in compression is reduced following a linear softening law once its strength is reached. The effect of imperfections such as initial ﬁbre misalignment (q0 ) is also considered. The failure envelopes obtained (ﬁgure 11) show that ﬁbre kinking occurs in composites with large ﬁbre initial misalignments or high ﬁbre compressive strengths, while ﬁbre fracture can occur for materials with less signiﬁcant ﬁbre misalignments or lower ﬁbre compressive strength XCf (leading in these cases to bimodal failure envelopes as in ﬁgure 9a,b). Figure 12a,b shows that the FE model is able to reproduce accurately the different trends found experimentally [10,11]. For ﬁbre kinking, the micromechanical FE models also give the width of the localized failure zone, i.e. the width of the kink band (w) non-dimensionalized by the ﬁbre diameter (ff ; ﬁgure 12c). For the speciﬁc material properties used [4], the models predict that failure only localizes into a kink band for shear stresses lower than approximately 75 MPa; for higher shear stresses, failure therefore corresponds to ﬁbre–matrix splitting. Despite the signiﬁcant change in localization predicted by the FE models, the transition from ﬁbre kinking to ﬁbre–matrix splitting is not apparent in the numerical failure envelopes; as, for example, in the envelopes of ﬁgure 11, which correspond to the predictions of ﬁgure 12c. This also reﬂects the experimental ﬁndings in the study of Jelf & Fleck [10], shown in ﬁgure 12a, where the transition from ﬁbre kinking to ﬁbre– matrix splitting was reported for shear stresses greater than 50 MPa without any change in the trend of the failure envelope. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1879 Longitudinal compressive failure of CFRP 40 FE, q0= 0.5° FE, q0= 1.5° [11], set 1 [11], set 2 LaRC05 (c) 160 120 80 200 w/ff (b) 80 t12 (MPa) FE, q0 = 4° [10] LaRC05 t12 (MPa) (a) 100 40 –1600 –1200 –800 s11 (MPa) –400 0 –1000 –800 –600 –400 –200 s11 (MPa) 0 0 20 40 60 t12 (MPa) 80 100 Figure 12. (a,b) Numerical predictions for bimodal failure envelopes against experimental data [10,11]. (c) Width of a kink band during longitudinal compression with in-plane shear, as a function of applied shear stress [4]. For materials that exhibit a bimodal failure envelope for longitudinal compression combined with in-plane shear, failure under pure longitudinal compression (t12 = 0) is predicted as ﬁbre compressive failure, independent of ﬁbre kinking. In ﬁgure 3, it is also observed that failure of carbon ﬁbres (within a kink band) results from the formation of shear bands within the ﬁbre at angles approximately 45◦ to the ﬁbre axis, and it was therefore inferred in §2a(i) that ﬁbre fracture was a shear-dominated process. The numerical predictions and experimental observations of ﬁbre compressive failure appear to have the same origins, and §2c will discuss further how this relates to macroscopic shear failure in longitudinal compression. (iii) Analytical modelling Several theories can be used for failure predictions under combined longitudinal compression and in-plane shear; some results from these theories are shown in ﬁgure 1c. In this section, an analytical model capable of generating such envelopes is presented [14]. The experimental observations show that kink-band initiation results from the formation of matrix microcracks and splits in the inter-ﬁbre region (ﬁgure 2). Therefore, the formulation of the present model is based on the hypothesis that the strength of the composite associated with ﬁbre kinking is reached when the strain energy released per unit area of crack generated between an undamaged state and a damaged state is equal to the energy required to create the cracks (fracture energy). To calculate the energy balance, a two-dimensional model with unit thickness is used. The two-dimensional model consists of a representative element of the kink band, i.e. a ﬁbre of length w (kink-band width) embedded in a matrix (ﬁgure 13a), onto which compressive (P) and shear (S ) loads are applied. The bending contribution of the ﬁbres is neglected and the resin is assumed to carry only shear stresses (t). The model can also account for ﬁbre misalignment through the introduction of the variable q0 as well for a nonlinear response in shear. Further details on the derivations can be found in Gutkin et al. [14]. The model leads to an interaction between longitudinal and shear loading as shown in ﬁgures 13b and 14. Figure 13b shows that the analytical predictions compare well against the results from the micromechanical FE model presented Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1880 S. T. Pinho et al. (b) 100 q rm d fo ban ink- P ation k S analytical: linear shear-driven fibre compressive failure w t t S analytical: nonlinear FE: nonlinear elasto-plastic –1500 –1000 s11 (MPa) 50 40 30 FE: elastic perfectly plastic –2000 P 90 80 70 60 t12 (MPa) q0 (a) 20 10 –500 0 Figure 13. (a) Equilibrium of a ﬁbre under a longitudinal compressive force and a shear force at each end, as well as a distributed shear force across the length. (b) Comparison between analytical (§2b(iii)) and numerical (§2b(ii)) failure envelopes for linear and nonlinear shear responses [14]. –1600 –1200 40 [11], set 2 [11], set 1 160 analytical: q0 = 2.6° SL = 125 MPa 120 80 analytical: q0 = 1° SL = 94 MPa analytical: q0 = 2.5° SL = 75 MPa –800 – 400 s11 (MPa) 0 –1000 –800 –600 – 400 –200 t12 (MPa) analytical: q0 = 2.1° SL = 75 MPa (b) 80 [10] t12 (MPa) (a) 40 0 s11 (MPa) Figure 14. Failure envelopes predicted by the analytical model (§2b(iii)) [14] against experimental data [10,11]. in §2b(ii) and ﬁgure 14 shows a good agreement of the analytical model against experimental results from the literature [10,11]. In ﬁgure 14b, the different levels of initial ﬁbre misalignment corresponding to different datasets are suggested as the reason underlying the apparent scatter observed experimentally. (c) Another failure mode for longitudinal compression: shear-driven ﬁbre compressive failure (i) Experimental observations Another failure mode—brittle shear fracture at 45◦ to the ﬁbres (ﬁgure 15)— was observed experimentally [8] through developments that allowed for a greater control over the loading process during initiation. For different layups and loading rigs, the 45◦ fracture plane is seen to form, propagate and only then degenerate into a kink band. The transition between shear-driven ﬁbre compressive failure and ﬁbre kinking is particularly sharp (ﬁgure 15). Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1881 Longitudinal compressive failure of CFRP (a) (b) kink-band tip (c) A b = 25° b = 45° A x y 1mm (c) shear-driven fibre transition (d) kink band compressive failure (d ) 2 1 50 µm 100 µm (e) (f) radial patterns ‘T’ neutral axis ‘C’ 15 kV ×11 000 1 µm 19 20 SEI 15 kV ×7 000 2 µm 18 20 SEI Figure 15. (a–d) Shear-driven ﬁbre compressive failure as an independent failure mode that eventually leads to kink-band formation. (e) Bending failure of a ﬁbre during kink-band formation. (f ) Broken ﬁbre in the shear-driven ﬁbre compressive failure region [8]. It is hypothesized that this type of failure may be more common than expected, given that its occurrence is easily masked or lost because of the catastrophic and crushing nature of compressive failure. The different failure modes leave different features on the cross section of the broken ﬁbres (ﬁgure 15e, f ). For instance, ﬁbre ends at the kink-band edges show a typical bending failure pattern, with Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1882 S. T. Pinho et al. 120 Soden et al. (1994) inputs model 100 60 40 XCf = 2500 MPa 20 XCf = 1300 MPa –1800 t12 (MPa) 80 transition: compressive shear failure to kinking –1600 –1400 –1200 –1000 –800 –600 –400 –200 0 s11 (MPa) Figure 16. Complete failure envelope prediction for combined longitudinal compression and in-plane shear [14]. tensile (label ‘T’ in ﬁgure 15e) and compressive (label ‘C’ in ﬁgure 15e) failures separated by a neutral axis, while for shear-driven ﬁbre compressive failure, the ﬁbre ends are smooth and show signiﬁcant abrasion (ﬁgure 15f ). (ii) Modelling The modelling of shear-driven ﬁbre compressive failure can be easily achieved using a maximum shear criterion in the ﬁrst instance, resulting in combined envelopes for shear-driven ﬁbre compressive failure/ﬁbre kinking/splitting as shown in ﬁgure 16. 3. Compressive failure in woven composites (a) Experimental observations Experimental studies analogous to those on UD composites were carried out for woven composites [15]. Different reinforcement architectures were tested under compression: 2 × 2 twill and ﬁve-harness (5H) satin. Kinking was identiﬁed as the mechanism responsible for the failure of the load-aligned tows (ﬁgure 17a). The latter has a structural role within the reinforcement architecture, highlighted in ﬁgure 17b, where tows are observed to fail individually. Moreover, the reinforcement architecture was seen to affect the failure morphology and immediate sequence of events [15]. One of the observed differences in failure morphology is highlighted in ﬁgure 18; while 2 × 2 twill tows tended to fail at the centre of the crimp region (d ≈ 0), 5H satin tows failed systematically at a distance d = 0 from it. In a two-dimensional woven laminate, shifting between adjacent layers is usually not controlled, leading to a random conﬁguration (ﬁgure 19a). Upon Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 Longitudinal compressive failure of CFRP 1883 1 mm (a) (b) 3 mm 100 µm Figure 17. (a) Tow failed by kinking; (b) several tows failing individually [15]. (a) (b) d d 0 d d 0 Figure 18. Differences in failure location between different reinforcement architectures: 2 × 2 twill and 5H satin [15]. (a) 5H satin: tows failed at a distance d = 0 from the centre of the crimp region. (b) 2 × 2 twill: tows failed at a distance d ≈ 0 from the centre of the crimp region. (a) (b) (c) Figure 19. Cross sections of (a) random-stacked, (b) IP and (c) OP laminates. (Online version in colour.) Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1884 S. T. Pinho et al. (a) transverse tow cracking kink band matrix cracking (b) equivalent regions on adjacent layers splitting delamination fibre breaks Figure 20. Longitudinal compression in a 2 × 2 twill composite [15]. (a) Random stacking and (b) IP stacking. (Online version in colour.) compression, adjacent layers will naturally interact. This interaction, namely the out-of-plane support provided by the adjacent layers, was also investigated. Several specimens were produced with carefully aligned adjacent layers in an IP conﬁguration, i.e. all load-aligned tows of adjacent layers are IP (ﬁgure 19b). Figure 20 shows that the failure morphology changes signiﬁcantly with the support provided by the adjacent layers. As highlighted previously, tows behave as structural elements within the reinforcement architecture; under compression, the out-of-plane support provided by the adjacent layers affects the bending of the tows and consequently the failure morphology. This effect was also seen to be a function of the reinforcement architecture [15]. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1885 Longitudinal compressive failure of CFRP (a) (b) 2 1 2 1 Figure 21. At the microscale, compressive damage starts with microcracking/plasticity of the matrix, leading to splitting (1) at the interface of the load-aligned tows and/or within the tows. The ﬁrst ﬁbre failures (2) occur soon after. Further loading leads to the development of kink bands. (a) 5H satin and (b) 2 × 2 twill. At the microscale, compressive failure of woven composites occurs according to the process previously described for UD composites: microcracking/plasticity of the matrix between ﬁbres (within the tows or at the interface between tows and pure matrix regions) leading to kinking/splitting (ﬁgure 21). (b) Numerical and analytical modelling An FE model of a 2 × 2 twill reduced unit cell (rUC) was developed [16] (ﬁgure 22a). The rUC used is the smallest possible domain that can be used to analyse a 2 × 2 twill geometry, while applying the correct periodic boundary conditions both in-plane and out-of-plane [19]. In the out-of-plane direction, two sets representing different cases of out-of-plane support were applied: (i) in-phase (IP), where all load-aligned tows of adjacent layers are IP, and (ii) out-of-phase (OP), where all load-aligned tows of adjacent layers are OP (ﬁgure 19b,c), respectively. These two cases deﬁne practical limits of support that any layer can have within a laminate, where adjacent layers are randomly shifted. The tows are modelled as an orthotropic material, with the material orientations following the central path of the tow. The matrix is considered to be an elasto-plastic material and its response is modelled using a linear Drucker– Prager plasticity model. Additionally, the debonding between tows and matrix is accounted for and modelled through the deﬁnition of cohesive contact. The longitudinal compressive failure is predicted using a kinking model [20], developed for UD materials, applied at the tow level. The use of such a model to predict the compressive failure of woven composites is in agreement with what is found Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1886 (a) tows S. T. Pinho et al. (b) matrix tows region A region B 2 y0 1 LA LB Figure 22. (a) Finite-element model of a 2 × 2 twill rUC. (b) Analytical model; the geometry of the tow is approximated by a sinusoidal beam connected with a straight beam, regions A and B, respectively [16–18]. (Online version in colour.) experimentally, where compressive failure is seen to occur by kinking of the loadaligned tows (ﬁgure 17). The material is assumed to fail when failure of the load-aligned tows is detected using the referred criterion. With the insight gathered from both experimental and numerical investigations, an analytical model was also developed [17,18] (ﬁgure 22b). It consists of an Euler–Bernoulli beam supported by an elastic foundation. The beam represents the load-aligned tow and is regarded as a UD composite. The elastic foundation provides both normal and torsional support, and its properties are derived from kinematic models that account for: weave effect, case of support provided by the adjacent layers (IP or OP), and elastic properties of the tows and matrix (ﬁgure 23). The weave effect (ﬁgure 23a) is accounted for by considering that the IP adjacent tows affect the deﬂection of each other through the shearing of the matrix connecting them. The latter is obtained by realizing that the deﬂection of adjacent tows can be related, taking into account that equivalent positions in adjacent tows displace in the same fashion [19]. Having determined the shearing of the connecting matrix, the distributed load exerted in a given tow by the adjacent tows can be approximated by pweave (x) = 2 (y0 + t¯tow ) Gm v(x), g (3.1) where y0 is a geometrical parameter (ﬁgure 22b), t¯tow represents the average tow thickness over the cross section of the tow, g is the gap between adjacent tows, Gm is the shear modulus of the matrix and v(x) is the deﬂection of the tow. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1887 Longitudinal compressive failure of CFRP (a) Tl Tc g Tr vc vl cl (b) vr cr (c) undeformed undeformed deformed deformed dv dv dv t tow hTop–2dv hTop dv ttow du h hBot+2dv hBot dv dv dx dx Figure 23. Kinematic models used to derive the properties of the elastic foundation [17,18]. (a) Weave effect: shearing of the matrix connecting in-plane adjacent tows (of the same woven layer); vl , vc and vr represent the deﬂections of the tows Tl , Tc and Tr , respectively; gcl and gcr are the shear strains of the matrix connecting Tc to Tl and Tr . (b) In-phase: shearing of the material between load-aligned tows of adjacent layers. (c) Out-of-phase: straining (through-thickness direction) of the material between tows of adjacent layers. (Online version in colour.) The kinematic model that accounts for the IP support is illustrated in ﬁgure 23b. In this case, the support is essentially provided by the shearing of the material (matrix and transverse tows) between load-aligned tows. Assuming that all load-aligned tows from adjacent layers displace in an identical fashion (ﬁgure 23b), the shear strain of the material between tows can be obtained from Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1888 S. T. Pinho et al. geometrical considerations, as a function of the tow deﬂection. Knowing the shear strain, the shear stress applied to a given tow can be determined by t¯tow dv , (3.2) tIP (x) = Gh 1 + h dx where Gh is the modulus of the material between tows, homogenized using the rule of mixtures, and h is the average thickness of the material between tows. Additionally, the gradient of equation (3.2) leads to a direct pressure applied to the tow given by dt (3.3) p(x) = − hbtow , dx where btow is the width of the tow. This gradient is obtained from the equilibrium of the material between tows [18]. In the OP conﬁguration (ﬁgure 23c), the support is mainly provided by the straining of the material between load-aligned tows because of their deﬂection in opposite directions. Similar to the IP case, the strain of the region between tows can be obtained from geometrical considerations (ﬁgure 23c). Knowing the strain, the pressure padj , applied by the load-aligned tows of the adjacent layers, is obtained by: Top Top EhBot (1 − nhBot ) Eh (1 − nh ) + , (3.4) padj = 2v(x)btow Top Bot Bot Top (1 − nh )(1 − 2nh )h Top (1 − nh )(1 − 2nh )h Bot Top/Bot Top/Bot and nh are the homogenized Young’s moduli and Poisson’s where Eh ratios, and h Top/Bot is the distance between the adjacent tows. The superscripts ‘Top’ and ‘Bot’ refer to the regions above and below a given tow, respectively. Finally, the governing differential equation is derived in a general fashion from the analysis of the equilibrium of a beam element (ﬁgure 24): 2 d2 v(x) d4 v(x) 2 2 2 d y0 (x) + l v(x) = −l , + l 1-IP/OP 2-IP/OP 3 dx 4 dx 2 dx 2 (3.5) where li-IP/OP are a function of the case of support (IP/OP) considered, and y0 (x) is the initial shape of the tow. Figure 25a compares the numerical and analytical results for the shear along the tow centreline obtained for the IP case. The good agreement indicates that the analytical model developed captures well all the key features of the weave response under compression. Figure 25b compares the numerical and analytical compressive strength predictions with the experiments. The numerical and analytical predictions are obtained by averaging the strength predictions for the IP and OP cases. The analytical and numerical models show accurate strength predictions (within the scatter of the experiments). Nevertheless, the numerical model shows better agreement with experiments. This is attributed to the more accurate stress ﬁelds obtained numerically and to the modelling of the nonlinear response of the matrix. It is worth highlighting that the nonlinear material response can be included in the analytical model. However, the governing differential equation would have to be solved iteratively or numerically, thus Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1889 Longitudinal compressive failure of CFRP p t P M+ S dM dx dx dy P M S+ dS dx dx y dx x Figure 24. Equilibrium of a beam element. P is the load applied; M and S represent the moment and shear force; p and t denote the pressure and shear applied to the tow by the elastic foundation [17,18]. (a) (b) –700 –500 100 numerical analytical 50 s11 (MPa) t12LCS (MPa) –600 0 –50 0 0.5 1 x/L –400 –300 –200 –100 0 analytical numerical experimental Figure 25. Comparison between the numerical, analytical and experimental results [16–18]. (a) Analytical and numerical predictions for the shear along the centre of the tow (IP) given in the local coordinate system aligned with the centreline of the tow; homogenized strain applied, 31 = −0.008. (b) Comparison between the analytical, numerical and experimental results for the compressive strength. In the analytical and numerical predictions, the min/max limits of the error bars correspond to the results obtained with IP/OP cases, respectively. compromising the simplicity of the proposed model. The analytical model has runtime of less than 2 s in its current form. This is extremely beneﬁcial when performing parametric or stochastic studies. 4. Compressive failure in recycled composites (a) Introduction In recent decades, the exponential increase in the use of carbon-ﬁbre-reinforced polymer (CFRP) has motivated the development of recycling technologies for the ever-increasing amount of CFRP waste produced. It is suggested that recycling Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1890 S. T. Pinho et al. fibre bundle dispersed phase 500 µm Figure 26. Recycled composite with a multi-scale structure consisting of ﬁbre bundles in a shortﬁbre-reinforced matrix [22]. CFRP can bring environmental and economic beneﬁts over the traditional methods of landﬁlling and incineration. Recent studies [21] have also shown that recycled (r-) CFRP can replace traditional materials, with weight savings in selected structural applications, such as non-safety-critical components in the aeronautical and automotive industries currently manufactured with aluminium or glass-ﬁbre. Recycled composites are manufactured by re-impregnating recycled carbon ﬁbres with a new resin. The recycling step typically consists of a thermal or chemical process to break down the matrix and release the valuable carbon ﬁbres, either from end-of-life components or from manufacturing waste. Owing to the reprocessing, recycled composites present distinct features from those of their virgin precursors, namely regarding the micromechanical properties of constituents (ﬁbres and interface) and the reinforcement architecture. Such speciﬁcities require the development of dedicated material models and design methods for rCFRPs. However, despite their signiﬁcant differences, the mechanisms involved in the compressive failure of recycled composites share many features with UD and woven composites (detailed in §§2 and 3). This section discusses similarities and differences between the compressive failure of two types of rCFRP and their virgin counterparts. (b) Short-ﬁbre recycled composites Most rCFRPs have a short-ﬁbre randomly oriented architecture. However, in contrast to most virgin short-ﬁbre composites, the recyclates typically present a multi-scale reinforcement architecture, with individually dispersed ﬁbres and ﬁbre bundles; these bundles are held together by residual matrix not removed during the recycling (ﬁgure 26). Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1891 Longitudinal compressive failure of CFRP (a) (b) complementary shear band shear band shear band b ~ 20° b ~ 54° 300 µm (c) 500 µm (d ) tow bending kink band 300 µm 200 µm Figure 27. Compressive failure of short-ﬁbre rCFRPs with ﬁbre bundles [22]. (a) Shear band at initial stage (b ≈ 20◦ ). (b) Shear band at ﬁnal failure (b ≈ 54◦ ). (c) Bending of an isolated ﬁbre bundle. (d) Kink band in a supported ﬁbre bundle. Compressive failure of recycled composites with such architecture is complex [17]. In areas with no bundles (ﬁgure 27a,b), a fracture plane starts to form at low angles (b < 20◦ ) and then rotates up to approximately 54◦ through plastic deformation of the matrix. In areas with bundles, the failure process resembles the failure of tows in woven composites: isolated bundles fail by bending (ﬁgure 27c), while kink bands are formed whenever neighbouring bundles provide sufﬁcient support (ﬁgure 27d). (c) Woven recycled composites To further investigate the effect of ﬁbre recycling on the performance of rCFRPs, samples of out-of-date woven prepreg were recycled under different pyrolysis conditions, and re-impregnated into woven rCFRPs, mimicking the architecture of the virgin composite (the 5H satin analysed in §3). Both virgin and recycled materials were characterized at the ﬁlament and composite levels [23]. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1892 S. T. Pinho et al. (a) (b) rCF (c) rCFRP rCFRP retention (%) 100 80 60 40 20 0 ET XT ET XT EC XC (d ) kink bands transverse tow cracking 250 µm Figure 28. Mechanical response of a woven rCFRP: the compressive performance at the recycled composite level is shown to be insensitive to ﬁbre strength degradation, occurring in the most aggressive recycling conditions. (a) Recycled ﬁbre properties: retention of modulus (ET ) and strength (XT ) relative to virgin ﬁbre. (b) Recycled CFRP tensile properties: retention of modulus (ET ) and strength (XT ) relative to virgin composite. (c) Recycled CFRP compressive properties: retention of modulus (EC ) and strength (XC ) relative to virgin composite. (d) Morphology of compressive failure. In spite of the severe ﬁbre strength degradation that occurs during the most aggressive reclamation cycles, ﬁbre stiffness remained relatively unchanged (ﬁgure 28a); these results at the ﬁlament level were directly replicated on the tensile performance of the composite (ﬁgure 28b). However, the compressive strengths of the rCFRP and virgin CFRP were statistically the same (ﬁgure 28c), and the failure features are remarkably similar (ﬁgure 28d). The fact that the compressive strength of a woven CFRP is independent of its tensile strength—at both ﬁbre and composite levels—suggests that ﬁbre kinking is indeed governed by the failure of the resin or ﬁbre–matrix interface, rather than by the tensile failure of the ﬁbres themselves. Moreover, it was shown that rCFRPs can assume unique combinations of mechanical properties, underlining the need for speciﬁc models and design methods for these materials. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 Longitudinal compressive failure of CFRP 1893 5. Overall discussion It is found that there are two competing mechanisms for longitudinal compressive failure in UD composites: the widely documented kink-band formation (also referred to in the literature as microbuckling), and (the much less documented) shear failure of the ﬁbres at an approximately 45◦ angle to the loading direction. Both mechanisms can be described analytically by resolving the stress ﬁeld at the ﬁbre and matrix level, with the ﬁbres idealized as beams, leading to predictions for failure stresses and morphologies in agreement with experimental observations. Despite their more complex architecture, woven composites under longitudinal compression exhibit similar failure morphologies to those in UD composites, thus suggesting similar mechanisms (compare ﬁgures 2 and 15 for UD to ﬁgures 20 and 21 for woven). The analytical treatment is in this case made more difﬁcult not only by the morphology of the weave, but also by the uncertainty related to the exact stacking conﬁguration, and hence through-the-thickness support provided to a given layer. Analytical models for extremes of this support (IP and OP stacking), whereby the tows are idealized as beams, are however shown to accurately capture the stress ﬁelds within the tows. In turn, combining these stress ﬁelds in the tows with models for ﬁbre kinking originally developed for UD composites lead to compressive strength predictions in agreement with experiments and FE results. This conﬁrms that the failure mechanisms for UD and woven composites under longitudinal compression are intrinsically physically similar. Recycled composites that preserve the original woven architecture of the weave hold the potential to provide further insight into the validity of analytical models. In fact, a common denominator for ﬁbre kinking models (those presented herein but also most in the literature) is that strength depends strongly on the strength/toughness of the matrix and interface, but not on the strength of the ﬁbres. By varying the thermo-chemical parameters of the recycling process, it is possible to manufacture different recycled woven composites that are essentially the same, but with varying ﬁbre strength. Experimentally, it was found that reducing the ﬁbre strength by approximately 80 per cent has virtually no effect on the compressive strength of the composite (ﬁgure 28a–c), while it has, obviously, dramatic effects in tension. Additionally, the morphology of the failure process in these woven composites with much lower tensile ﬁbre strength (ﬁgure 28d) is remarkably similar to that in virgin woven composites (ﬁgures 20 and 21). This ﬁnding, obtained using recycled composites, provides a strong indication for the wide range of applicability of the models currently available for ﬁbre kinking in virgin UD and woven composites. Recycled composites also present a wealth of novel reinforcement architectures; this offers new challenges for both understanding and modelling their compressive failure. One such type of architecture consists of a matrix reinforced by randomly dispersed short ﬁbres and bundles of different dimensions (ﬁgure 26), effectively providing reinforcement to the matrix over several scales. The bundles in these materials exhibit failure mechanisms similar to those in UD (compare ﬁgure 27 with ﬁgures 2 and 15) and woven composites (compare ﬁgure 27 with ﬁgures 20 and 21). This suggests that analytical models for compressive failure of these novel materials ought to be based on the same principles adopted for the traditional architectures. Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 1894 S. T. Pinho et al. 6. Conclusions The ﬁrst part of this paper presents experimental and micromechanical FE studies, which were conducted with the aim of developing analytical models for longitudinal compressive failure in UD composites. Predictions from such models are shown to compare favourably with the numerical and experimental results. The existence and importance of a shear-driven ﬁbre compressive failure mode under longitudinal compression is highlighted, as it is shown to be critical for explaining different trends observed in experimental failure envelopes. Woven composites show some similarities to UD composites in their longitudinal compressive failure modes. In particular, it is shown that, once the stress ﬁeld is resolved in the tows, ﬁbre kinking models originally developed for UD composites can be successfully applied to woven composites. However, in obtaining the stress ﬁeld in the tows, woven composites also show some added complexity, such as the dependence of the failure process on the through-thethickness support provided by the adjacent layers. Experimental results using woven composites with very weak recycled ﬁbres suggest that the longitudinal compressive strength of woven composites does not depend on tensile ﬁbre strength. This ﬁnding is in agreement with the models presented, which do not depend on that variable for ﬁbre kinking. The similarities in the longitudinal compressive failure processes of different materials, regardless of their exact microstructure, suggest that knowledge and experience gathered in recent decades in analysing advanced composites appears to be very valuable for the analysis of novel types of composites, such as recycled composites with multi-scale ﬁbre bundle reinforcement. Different parts of this work were funded by EPSRC, DSTL, Airbus and Renault F1 (EP/E0Z3169/1), as well as FCT (SFRH/BD/36636/2007and SFRH/BD/44051/2008). References 1 Rosen, B. W. 1965 Mechanics of composite strengthening. In Fiber composite materials, ch. 3, pp. 37–75. Metals Park, OH: American Society for Metals. 2 Argon, A. S. 1972 Fracture of composites. In Treatise on materials science and technology, vol. 1, pp. 79–114. New York, NY: Academic Press. 3 Pimenta, S., Gutkin, R., Pinho, S. T. & Robinson, P. 2009 A micromechanical model for kinkband formation: Part I. Experimental study and numerical modelling. Compos. Sci. Technol. 69, 948–955. (doi:10.1016/j.compscitech.2009.02.010) 4 Gutkin, R., Pinho, S. T., Robinson, P. & Curtis, P. T. 2010 Micro-mechanical modelling of shear-driven ﬁbre compressive failure and of ﬁbre kinking for failure envelope generation in CFRP laminates. Compos. Sci. Technol. 70, 1214–1222. (doi:10.1016/j.compscitech. 2010.03.009) 5 Budiansky, B., Fleck, N. A. & Amazigo, J. C. 1998 On kink-band propagation in ﬁber composites. J. Mech. Phys. Solids 46, 1637–1653. (doi:10.1016/S0022-5096(97)00042-2) 6 Fleck, N. A., Jelf, P. M. & Curtis, P. T. 1995 Compressive failure of laminated and woven composites. J. Compos. Technol. Res. 17, 212–220. (doi:10.1520/CTR10485J) 7 Soutis, C., Fleck, N. A. & Smith, P. A. 1991 Failure prediction technique for compression loaded carbon ﬁbre–epoxy laminate with open holes. J. Compos. Mater. 25, 1476–1498. (doi:10.1177/002199839102501106) 8 Gutkin, R., Pinho, S. T., Robinson, P. & Curtis, P. T. 2010 On the transition from sheardriven ﬁbre compressive failure to ﬁbre kinking in notched CFRP laminates under longitudinal compression. Compos. Sci. Technol. 70, 1223–1231. (doi:10.1016/j.compscitech.2010.03.010) Phil. Trans. R. Soc. A (2012) Downloaded from http://rsta.royalsocietypublishing.org/ on October 29, 2018 Longitudinal compressive failure of CFRP 1895 9 Pimenta, S., Gutkin, R., Pinho, S. T. & Robinson, P. 2009 A micromechanical model for kink-band formation: Part II. Analytical modelling. Compos. Sci. Technol. 69, 956–964. (doi:10.1016/j.compscitech.2009.02.003) 10 Jelf, P. M. & Fleck, N. A. 1994 The failure of composite tubes due to combined compression and torsion. J. Mater. Sci. 29, 3080–3084. (doi:10.1007/BF01117623) 11 Soden, P. D., Hinton, M. J. & Kaddour, A. S. 2002 Biaxial test results for strength and deformation of a range of E-glass and carbon ﬁbre reinforced composite laminates: failure exercise benchmark data. Compos. Sci. Technol. 62, 1489–1514. (doi:10.1016/S0266-3538(02) 00093-3) 12 Yerramalli, C. S. & Waas, A. M. 2003 A failure criterion for ﬁber reinforced polymer composites under combined compression–torsion loading. Int. J. Solids Struct. 40, 1139–1164. (doi:10.1016/S0020-7683(02)00649-2) 13 Michaeli, W., Mannigel, M. & Preller, F. 2009 On the effect of shear stresses on the ﬁbre failure behaviour in CFRP. Compos. Sci. Technol. 69, 1354–1357. (doi:10.1016/j.compscitech. 2008.09.024) 14 Gutkin, R., Pinho, S. T., Robinson, P. & Curtis, P. T. 2011 A ﬁnite fracture mechanics formulation to predict ﬁbre kinking and splitting in CFRP under combined longitudinal compression and in-plane shear. Mech. Mater. 43, 730–739. (10.1016/j.mechmat.2011.08.002) 15 de Carvalho, N. V., Pinho, S. T. & Robinson, P. 2011 An experimental study of failure initiation and propagation in 2D woven composites under compression. Compos. Sci. Technol. 71, 1316–1325. (doi:10.1016/j.compscitech.2011.04.019) 16 de Carvalho, N. V., Pinho, S. T. & Robinson, P. Submitted. Numerical modelling of 2D woven composites: biaxial loading. Compos. Part A: Appl. Sci. Manuf. 17 de Carvalho, N. V., Pinho, S. T. & Robinson, P. Submitted. Analytical modelling of the compressive and tensile response of 2D woven composites. Compos. Struct. 18 Pinho, S. T., de Carvalho, N. V. & Robinson, P. 2011 Analytical model for the compressive response of 2D woven composites. In Proc. 5th Int. Conf. on Composites Testing and Model Identiﬁcation (CompTest 2011), 14–16 February, Switzerland. Lausanne, Switzerland: Ecole Polytechnique Fédérale de Lausanne. 19 de Carvalho, N. V., Pinho, S. T. & Robinson, P. 2011 Reducing the domain in the mechanical analysis of periodic structures, with application to woven composites. Compos. Sci. Technol. 71, 969–979. (doi:10.1016/j.compscitech.2011.03.001) 20 Pinho, S. T., Darvizeh, R., Robinson, P., Schuecker, C. & Camanho, P. P. 2008 Material and structural response of polymer–matrix ﬁbre-reinforced composites. Compos. Sci. Technol. 21 Pimenta, S. & Pinho, S. T. 2011 Recycling carbon ﬁbre reinforced polymers for structural applications: technology review and market outlook. Waste Manage. 31, 378–392. (doi:10.1016/ j.wasman.2010.09.019) 22 Pimenta, S., Pinho, S. T., Robinson, P., Wong, K. H. & Pickering, S. J. 2010 Mechanical analysis and toughening mechanisms of a multiphase recycled CFRP. Compos. Sci. Technol. 70, 1713–1725. (doi:10.1016/j.compscitech.2010.06.017) 23 Pinho, S. T. & Pimenta, S. 2010 The potential of recycled carbon ﬁbres and composites for structural applications. In Global outlook for carbon ﬁbre, 29–30 September 2010, Valencia. Valencia, Spain: IntertechPira. Phil. Trans. R. Soc. A (2012)